VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

25 JUNE 2001

Charge Ordering and Spin Dynamics in NaV2 O5 B. Grenier,1 O. Cepas,2 L. P. Regnault,1 J. E. Lorenzo,3 T. Ziman,2 J. P. Boucher,4 A. Hiess,2 T. Chatterji,2 J. Jegoudez,5 and A. Revcolevschi5 1

Département de Recherche Fondamentale sur la Matière Condensée, SPSMS, Laboratoire de Magnétisme et de Diffraction Neutronique, CEA-Grenoble, F-38054 Grenoble cedex 9, France 2 Institut Laue Langevin, BP 156, F-38042 Grenoble cedex 9, France 3 Laboratoire de Cristallographie, CNRS, BP 166, F-38042 Grenoble cedex 9, France 4 Laboratoire de Spectrométrie Physique, Université J. Fourier Grenoble I, BP 87, F-38402 Saint Martin d’Hères cedex, France 5 Laboratoire de Physico-Chimie de l’Etat Solide, Université Paris-Sud, Bât 414, F-91405 Orsay cedex, France (Received 23 June 2000) We report high-resolution neutron inelastic scattering experiments on the spin excitations of NaV2 O5 . Below Tc , two branches with distinct energy gaps are identified. From the dispersion and intensity of the spin excitation modes, we deduce the precise zigzag charge distribution on the ladder rungs and the corresponding charge order: Dc 艐 0.6. We argue that the spin gaps observed in the low-T phase of this compound are primarily due to the charge transfer. DOI: 10.1103/PhysRevLett.86.5966

The low dimensional inorganic compound NaV2 O5 undergoes a phase transition at Tc 苷 34 K [1] associated with both a lattice distortion [2] and the opening of an energy gap to the lowest triplet spin excitations [3]. While the nature of the low-T phase in NaV2 O5 is not fully understood it is clear that, unlike CuGeO3, the spin-Peierls model does not apply simply to this compound [4]. The spin gap may result from charge order (CO) rather than the lattice distortion [5]. Indeed, NMR measurements indicate two inequivalent vanadium sites below Tc , while there exists only one site above [6]. There has been no direct evidence for the connection between CO and a spin gap, nor to distinguish various conjectured spatial distributions of charge [5,7]. In this Letter, we present new results of neutron inelastic scattering (NIS) on the spin excitations in the low-T phase that can now resolve these issues. In NaV2 O5 , the vanadium ions have a formal valence of 4.51. Initially, this was proposed to correspond to an alternation of V41 ions, with a spin value S 苷 1兾2, and V51 ions with S 苷 0 [8]. At room temperature, NaV2 O5 is well described by a quarter-filled two-leg ladder system, with only one type of vanadium site V4.51 . From calculations of electronic structure [9,10], the strongest orbital overlaps are on the ladder rungs. One expects that the S 苷 1兾2 spins are carried by the V-O-V molecular bonding orbitals, with charge fully delocalized on two sites. As the energy of the antibonding orbital is much higher, it can be projected out, and above Tc , these spins, as they interact in the leg direction (k b axis), form an effective uniform quantum Heisenberg spin chain with interactions between chains that are both weaker and frustrated. At low temperatures, NMR shows this can no longer be so. On each rung, a charge transfer Dc may occur. Taking the average charge on vanadium sites to be 1兾2, the charges on the two vanadium sites on a rung are defined through n6 苷 共1 6 Dc 兲兾2. Two forms of CO can be considered [5], the in line, with the same charge transfer on each rung, 5966

0031-9007兾01兾86(26)兾5966(4)$15.00

PACS numbers: 71.45.Lr, 75.10.Jm, 75.40.Gb

and the zigzag with alternation in the charge along the ladders as shown in Fig. 1b. Recent x-ray diffraction measurements [11] established that the lattice structure below Tc consists of a succession of distorted and nondistorted ladders of vanadium ions (see Fig. 1a). Neglecting interladder diagonal couplings J⬜ , the ladders would behave magnetically as independent spin chains. For one ladder (chain 2 in Fig. 1a) distortions in the exchange paths both within the ladder and via neighboring ladders result in an alternation of the effective exchange coupling in the b directions, Jb1 and Jb2 . The ladders in which the rungs are distorted (chains 1 and 3), however, remain magnetically uniform as a mirror plane passes through each rung. A minimum magnetic model without CO would be a succession of alternating and uniform chains. An energy gap (expected to be small as it results primarily from the alternation in J⬜ ) would characterize the excitation branch of

a)

b)

J

Jb

J’1 A J’2 J b1

Jb1 Jb

b

B Jb1

Jb2 B

Jb2 (1)

(2)

(3)

(1)

J’3 A J J’4 b2 (2)

a

(3)

FIG. 1. (a) Simplified representation of distorted and nondistorted chains, chain 1 (or 3) and 2, respectively, with the J⬜ bond alternation between chains 1 and 2; (b) proposed charge order (large and small lobes represent large and small average charges) leading to a spin gap. The elementary translation (a, b) of this CO agrees with the observed periodicity of spin excitations.

© 2001 The American Physical Society

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

the alternating chains, and there would be no gap for the uniform chains. The initial NIS [3] found, however, two excitation branches, with the same gap at the antiferromagnetic (AF) point Eg1 苷 Eg2 艐 10 meV. To analyze these results, a recent spin model [12] used an explicit relation between the spin excitations and the CO. This model assumed a single gap and, as it implies zero intensity of one excitation branch, must be extended to explain the NIS data. A more precise determination of excitations in the low-T phase of NaV2 O5 is therefore crucial. In the present work, using high resolution, the dispersion of the excitations is reexplored in a wider part of the reciprocal space. Moreover, the evaluation of the structure factor, i.e., the (energy-integrated) intensity of each excitation mode, allows us to determine the charge transfer Dc . The single crystal (艐8 3 5 3 2 mm3 ) was grown by a flux method. The NIS measurements were performed at T # 4.2 K, on two thermal neutron three-axes spectrometers — IN8 and CRG/CEA-IN22 — at the Institut Laue-Langevin (ILL). On IN8, vertically focusing monochromator PG(002) and Cu(111) were used in conjunction with a vertically focusing analyzer PG(002) and horizontal collimations 600 -400 -600 . The final wave vector was kept fixed at kf 苷 4.1 Å21 . IN22 was operated at kf 苷 2.662 Å21 , with a PG(002) monochromator and a PG(002) analyzer used in a horizontal monochromatic focusing condition [resulting wave-vector resolution: dq 艐 0.03 r.l.u. (reciprocal lattice units)] with no collimation. The sample was installed in an “orange” ILL cryostat, with the scattering wave vector Q lying in the reciprocal (aⴱ , b ⴱ ) ladder plane. The two branches characterizing the low-energy excitations in NaV2 O5 have distinct energy gaps: Eg1 ﬁ Eg2 . This important result will be established when we consider the dispersions in the transverse a direction. First, however, we determine the dispersion in the leg direction (b axis). Examples of constant-energy scans obtained on IN8 as a function of Qb are displayed in Fig. 2a (wave-vector components are expressed in r.l.u.). Increasing the energy, one resolves the single peak seen at 10 meV into propagating modes (dashed lines), whose peak position is shown in Fig. 2b. They describe the dispersion of the elementary excitations in the b direction, near the AF chain wavevector component QbAF 共⬅ Qb 苷 0.5兲 . They are compared to a dispersion law characteristic of a gapped spin chain: q 2 2 E 2 兲 sin2 共2pQ 兲, where E and E共qb 兲 苷 Eg2 1 共Em b g g Em are the gap and maximum energies of the dispersion, respectively. For both Eg 苷 Eg1 , Eg2 (the solid and dashed lines, respectively), we evaluate Em 苷 93 6 6 meV. Compared to the prediction for a uniform Heisenberg chain, Em 苷 pJb 兾2, where Jb is the exchange in the chain, one obtains for the low-T phase, Jb 艐 60 meV. Second, we consider the dispersions in the aⴱ direction (i.e., along the rungs). A few examples of energy scans performed on IN22 at constant Q are reported in Fig. 3. In general, two peaks are observed. At a few Qa values, however, an extinction occurs. This extinction may

25 JUNE 2001

FIG. 2. IN8 data: (a) Constant-energy scans as a function of Qb . The full lines are the results of fits to the data, which take into account both the magnetic contributions (shown as the dashed lines) and the background (the dotted line); (b) energy dispersion in the b direction. The lines correspond to the two branches with gaps Eg1 and Eg2 .

concern one of the two modes, or the two modes simultaneously. The left and right panels report data obtained for QbAF 苷 0.5 and Qb 苷 1 (equivalent to the zone center of the AF chains QbZC ). As examples, we show for QbAF that the smallest energy difference between the two observed peaks is obtained for integer Qa values (here, Qa 苷 3), the largest one for half-integer values (Qa 苷 2.5), and an extinction of the two modes occurs at Qa 艐 1.75 (identical results have been obtained for Qb 苷 1.5). Surprisingly, at the chain zone center QbZC we found a small but nonzero intensity for the two excitation branches. The smallest energy difference between the two peaks is now obtained for half-integer values (here, Qa 苷 1.5). Extinction of one of the two modes is observed at Qa 苷 1 (on the high-energy mode) and at Qa 苷 2 (on the low-energy mode). For all the spectra recorded on IN22, the background (the dotted lines in Fig. 3) was carefully determined. Several procedures have been used involving data recorded at low and high temperatures (i.e., above Tc ). In Fig. 3a, for instance, the open dots used to define the background are obtained from measurements performed at 40 K [13] while

FIG. 3. IN12 data: Constant-Q scans as functions of energy. (a) At Qb ⬅ QbAF ; (b) at Qb ⬅ QbZC . The two arrows point to the positions expected for the two missing peaks. Curves are described in text.

5967

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

in Fig. 1b, it is determined from Qb scans performed at low temperature for different energies. For the analysis, we assume the two observed peaks to belong to two distinct contributions. Their unsymmetrical line shape is characteristic of gapped excitations undergoing a rapid energy dispersion (as established in Fig. 2b). In such a case, a dynamical response function (shown by the dashed lines in Fig. 3) is well suited to fitting, conveniently defined with only three parameters: the peak energy E1 共E2 兲 , an intensity factor A1 共A2 兲, and an energy damping G [14]. As G is mainly fixed by the resolution conditions, it is assumed to be the same for the two contributions (G 艐 0.4 0.8 meV). Together with the background, the agreement with the experiments, shown by the solid lines, is good. The values obtained for E6 as a function of Qa are shown in Fig. 4. We establish several new features. At both QbAF (open symbols) and QbZC (solid symbols), the transverse dispersion consists of two distinct excitation branches which never cross. This justifies our previous statement, namely, that there are two distinct energy gaps, Eg1 and Eg2 . In each branch, the periodicity is 2pQa : this is twice that previously determined. The two dispersions have the same amplitude, dJ 艐 1 meV but, remarkably, the upper and lower branches are out of phase, and there is phase inversion between branches at QbZC and QbAF . For each excitation AF branch, the corresponding structure factors, Sb6 共Qa 兲 and ZC Sb6 共Qa 兲 are evaluated by integrating the fitted dynamical response functions over a wide energy range (from 0 up to E 艐 300G). We estimate systematic error for varying the upper cutoff alters the results by at most 5%. The resulting values (dots and squares) are reported in Figs. 5a AF AF and 5b. The sums SbAF 共Qa 兲 苷 Sb1 共Qa 兲 1 Sb2 共Qa 兲 and ZC ZC ZC Sb 共Qa 兲 苷 Sb1 共Qa 兲 1 Sb2 共Qa 兲 are shown as the stars. The interpretation of these results is developed in three steps. First, the charge order: each spin is associated with an electronic wave function on the two sites of a rung that depends on n6 . The structure factors for the in-line

FIG. 4. Dispersion of the two excitation branches in the a direction at QbAF and QbZC . The curves are theoretical predictions fitted to the data (see text).

5968

25 JUNE 2001

and zigzag models are SQb 共Qa , v兲 苷 cos2 共pQa r兲 3 ˜ a 1 1 , Qb , v兲 and ˜ a , Qb , v兲 1 Dc2 sin2 共pQa r兲S共Q S共Q 2 ˜ a , Qb , v兲 1 Dc2 sin2 共p 3 SQb 共Qa , v兲 苷 cos2 共pQa r兲S共Q ˜ a 1 12 , Qb 1 12 , v兲, Qa r兲S共Q respectively, with v 苷 E兾h¯ and where r 苷 l兾a 艐 0.304 (l, rung length ˜ a , Qb , v兲 is the strucand a, lattice parameter), and S共Q ture factor for spins localized on the center of each rung [15]. From the ratios of intensities for different values of momentum, one can extract the charge transfer Dc inde˜ In particular, we verify that the pendent of the form of S. order cannot be in line but predictions agree with a zigzag order with Dc2 艐 0.35, i.e., Dc 艐 0.6. The agreement is particularly good for the sums SbAF 共Qa 兲 and SbZC 共Qa 兲. For the absolute intensities, we need an explicit form for S˜ which we take from the strongly dimerized limit (SDL), in which the wave function is simply a product of singlets on the stronger bonds. For the in-line model, for example, the SDL would give zero intensity at QbZC in contradiction with the observation (the data in Fig. 5b). The in-line model can be ruled out. In Figs. 5a and 5b, the predictions provided by the zigzag model (solid lines) are compared with the experimental total structure factors SbAF 共Qa 兲 and SbZC 共Qa 兲 (solid and open stars). In Fig. 5a, the agreement is obtained with no adjustable parameter except for an overall amplitude factor. Once this factor is determined, the results in Fig. 5b depend only on D2c . As can be seen, a good agreement is obtained for D2c 艐 0.35. The low-T phase of NaV2 O5 is very well described by the zigzag model, with a rather large charge transfer.

ZC AF FIG. 5. Structure factors Sb6 共Qa 兲 and Sb6 共Qa 兲 for the two magnetic branches in the a direction: (a) at QbAF ; (b) at QbZC . The solid and open stars represent the sums SbAF 共Qa 兲 and SbZC 共Qa 兲. The data are corrected from the V41 atomic form factor fV 41 , being all normalized at Qb 苷 0.5. The dot-dashed line gives the Qa dependence of fV 41 . The other curves are theoretical predictions compared to the experiments (see text).

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

Second, we consider the transverse dispersions. Later, we explain that the gap is induced by the CO. In fact, there are two distinct gaps because of the strucA tural distortions (implying distinct couplings Jb1,2 and B Jb1,2 as shown in Fig. 1b). Because of the CO, four different interchain exchange integrals must be considered, J10 , J20 , J30 , and J40 . The two branches (associated with the gaps Eg1 and Eg2 ) acquire a transverse disAF 苷 共Eg1 1 persion, described at QbAF and QbZC by Eb6 q

ZC 苷 共Eg1 2 Eg2 兲2 兾4 1 dJ 2 sin2共pQa 兲 and Eb6 q 共Eg1 1 Eg2 兲兾2 6 共Eg1 2 Eg2 兲2 兾4 1 dJ 2 cos2共pQa 兲, respectively, with dJ 苷 J10 2 J20 1 J30 2 J40 [15]. In Fig. 4, these predictions (solid and dashed lines) are compared to the data. Again, a very good agreement is obtained yielding the following evaluation Eg1 苷 10.1 6 0.1, Eg2 苷 9.1 6 0.1 and dJ 苷 1.2 6 0.1 meV. The dispersion gives directly the alternation in the interladder diagonal bonds dJ. If we assume it is dominated by the CO, we can also estimate the average from dJ 艐 J⬜ Dc2 [12] giving J⬜ 艐 2.4 meV. The structure factors can be calculated for each branch. Within the SDL approach, one obtains the contributions ZC AF Sb6 共Qa 兲 and Sb6 共Qa 兲 [16] shown by the dotted and dashed lines in Fig. 5. In Fig. 5b, the agreement with the data is rather good. In particular, the extinction phenomenon observed for each branch is well reproduced. In Fig. 5a, while the sum SbAF 共Qa 兲 is well described, we note a discrepancy between the SDL predictions and the AF AF individual structure factors Sb1 共Qa 兲 and Sb2 共Qa 兲. This difficulty could be explained as follows. As shown in Fig. 1b, two successive chains are not identical. A charge transfer giving different average valence on the chains will mix intensities at QbAF without affecting the fluctuations at QbZC in qualitative agreement with the observation [17]. Experimental supports for such a charge transfer would be useful. Our proposition for the charge ordering, i.e., the zigzag model sketched in Fig. 1a, and our estimate Dc 艐 0.6 are based on the total intensities. Finally, we consider the origin of the gap. As discussed in the introduction, the lattice distortion alone, in isolated ladders, cannot explain the presence of two energy gaps and their size. To analyze the effects of the diagonal couplings J⬜ , we refer to Fig. 1b. Each ladder is seen to be a succession of two distinct clusters (shown by ovals in the figure). By exact diagonalization of each cluster, using the effective parameters of a t-J model [10] and adding a potential imposing a charge transfer, we evaluated Jb1 and Jb2 as a function of Dc and the bond alternation d 苷 jJb1 2 Jb2 j兾共Jb1 1 Jb2 兲. For Dc 艐 0.6, the couplings underestimate the experimental value by a factor of about 2, but as the parameters calculated on the high temperature structure [10] and as such cluster calculations are rather crude, the agreement is satisfac-

Eg2 兲兾2 6

25 JUNE 2001

tory. The value obtained for the bond alternation can be considered as reasonable: d 艐 0.025 0.030. Then, using the experimental value Jb 艐 60 meV, one finds an energy gap Eg 艐 6 8 meV. This is in fairly good agreement with the experimental value Eg 艐 10 meV. This simple analysis supports the view that, in NaV2 O5 , the gaps are primarily due to the CO [18]. The lattice distortion plays a secondary role, explaining why two distinct branches are observed experimentally, and their separation. In our picture, the magnetic anisotropies are unnecessary [7]. In conclusion, the CO in NaV2 O5 is quantitatively determined by the present NIS measurements [19]. It explains also the energy gaps observed in the low-T phase of this compound.

[1] [2] [3] [4] [5]

[6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17]

[18]

[19]

M. Isobe and Y. Ueda, J. Phys. Soc. Jpn. 65, 1178 (1996). T. Chatterji et al., Solid State Commun. 108, 23 (1998). T. Yosihama et al., J. Phys. Soc. Jpn. 67, 744 (1998). S. G. Bompadre et al., cond-mat/9911298. M. Mostovoy and D. Khomski, cond-mat/9806215; A. Damascelli et al., Phys. Rev. Lett. 81, 918 (1998); P. Thalmeier and P. Fulde, Europhys. Lett. 44, 142 (1998); H. Seo and K. Fukuyama, J. Phys. Soc. Jpn. 67, 2602 (1998); J. Riera et al., Phys. Rev. B 59, 2667 (1999); A. I. Smirnov et al., ibid. 59, 14 546 (1999); H. Schwenk et al., ibid. 60, 9194 (1999); M. Lohmann et al., Phys. Rev. Lett. 85, 1742 (2000). T. Ohama et al., Phys. Rev. B 59, 3299 (1999). P. Thalmeier and A. N. Yaresko, Eur. J. Phys. B 14, 495 (2000). P. A. Carpy and J. Galy, Acta Crystallogr. Sect. B 31, 1481 (1975). H. Smolinski et al., Phys. Rev. Lett. 80, 5164 (1998). N. Suaud and M. B. Lepetit, Phys. Rev. B 62, 402 (2000). J. Lüdecke et al., Phys. Rev. Lett. 82, 3633 (1999). C. Gros and R. Valenti, Phys. Rev. Lett. 82, 976 (1999). Taking into account an estimated magnetic contribution for this temperature. T. E. Mason et al., Phys. Rev. Lett. 69, 490 (1992). O. Cepas, Ph.D. thesis, Université J. Fourier Grenoble I, France, 2000. The corresponding expressions agree with the sum rules SbAF 共Qa 兲 and SbZC 共Qa 兲 established above. In contrast, if we assume different values of Dc on two successive chains, the individual modes will mix at QbZC rather than at QbAF unlike what is observed. In T. Ohama et al., cond-mat/0003141, the CO proposed in model Z2 (Fig. 3) does not give rise to energy gaps; model Z3 provides a gap for only one out of two chains, and model Z1 is magnetically equivalent to ours (Fig. 1b). Other models assuming three different valence states (V41 , V4.51 , and V51 ) have been shown to be incompatible with our results: S. Trebst et al., Phys. Rev. B 62, R14 613 (2000); C. Gros et al., ibid. 62, R14 617 (2000), and references therein.

5969

PHYSICAL REVIEW LETTERS

25 JUNE 2001

Charge Ordering and Spin Dynamics in NaV2 O5 B. Grenier,1 O. Cepas,2 L. P. Regnault,1 J. E. Lorenzo,3 T. Ziman,2 J. P. Boucher,4 A. Hiess,2 T. Chatterji,2 J. Jegoudez,5 and A. Revcolevschi5 1

Département de Recherche Fondamentale sur la Matière Condensée, SPSMS, Laboratoire de Magnétisme et de Diffraction Neutronique, CEA-Grenoble, F-38054 Grenoble cedex 9, France 2 Institut Laue Langevin, BP 156, F-38042 Grenoble cedex 9, France 3 Laboratoire de Cristallographie, CNRS, BP 166, F-38042 Grenoble cedex 9, France 4 Laboratoire de Spectrométrie Physique, Université J. Fourier Grenoble I, BP 87, F-38402 Saint Martin d’Hères cedex, France 5 Laboratoire de Physico-Chimie de l’Etat Solide, Université Paris-Sud, Bât 414, F-91405 Orsay cedex, France (Received 23 June 2000) We report high-resolution neutron inelastic scattering experiments on the spin excitations of NaV2 O5 . Below Tc , two branches with distinct energy gaps are identified. From the dispersion and intensity of the spin excitation modes, we deduce the precise zigzag charge distribution on the ladder rungs and the corresponding charge order: Dc 艐 0.6. We argue that the spin gaps observed in the low-T phase of this compound are primarily due to the charge transfer. DOI: 10.1103/PhysRevLett.86.5966

The low dimensional inorganic compound NaV2 O5 undergoes a phase transition at Tc 苷 34 K [1] associated with both a lattice distortion [2] and the opening of an energy gap to the lowest triplet spin excitations [3]. While the nature of the low-T phase in NaV2 O5 is not fully understood it is clear that, unlike CuGeO3, the spin-Peierls model does not apply simply to this compound [4]. The spin gap may result from charge order (CO) rather than the lattice distortion [5]. Indeed, NMR measurements indicate two inequivalent vanadium sites below Tc , while there exists only one site above [6]. There has been no direct evidence for the connection between CO and a spin gap, nor to distinguish various conjectured spatial distributions of charge [5,7]. In this Letter, we present new results of neutron inelastic scattering (NIS) on the spin excitations in the low-T phase that can now resolve these issues. In NaV2 O5 , the vanadium ions have a formal valence of 4.51. Initially, this was proposed to correspond to an alternation of V41 ions, with a spin value S 苷 1兾2, and V51 ions with S 苷 0 [8]. At room temperature, NaV2 O5 is well described by a quarter-filled two-leg ladder system, with only one type of vanadium site V4.51 . From calculations of electronic structure [9,10], the strongest orbital overlaps are on the ladder rungs. One expects that the S 苷 1兾2 spins are carried by the V-O-V molecular bonding orbitals, with charge fully delocalized on two sites. As the energy of the antibonding orbital is much higher, it can be projected out, and above Tc , these spins, as they interact in the leg direction (k b axis), form an effective uniform quantum Heisenberg spin chain with interactions between chains that are both weaker and frustrated. At low temperatures, NMR shows this can no longer be so. On each rung, a charge transfer Dc may occur. Taking the average charge on vanadium sites to be 1兾2, the charges on the two vanadium sites on a rung are defined through n6 苷 共1 6 Dc 兲兾2. Two forms of CO can be considered [5], the in line, with the same charge transfer on each rung, 5966

0031-9007兾01兾86(26)兾5966(4)$15.00

PACS numbers: 71.45.Lr, 75.10.Jm, 75.40.Gb

and the zigzag with alternation in the charge along the ladders as shown in Fig. 1b. Recent x-ray diffraction measurements [11] established that the lattice structure below Tc consists of a succession of distorted and nondistorted ladders of vanadium ions (see Fig. 1a). Neglecting interladder diagonal couplings J⬜ , the ladders would behave magnetically as independent spin chains. For one ladder (chain 2 in Fig. 1a) distortions in the exchange paths both within the ladder and via neighboring ladders result in an alternation of the effective exchange coupling in the b directions, Jb1 and Jb2 . The ladders in which the rungs are distorted (chains 1 and 3), however, remain magnetically uniform as a mirror plane passes through each rung. A minimum magnetic model without CO would be a succession of alternating and uniform chains. An energy gap (expected to be small as it results primarily from the alternation in J⬜ ) would characterize the excitation branch of

a)

b)

J

Jb

J’1 A J’2 J b1

Jb1 Jb

b

B Jb1

Jb2 B

Jb2 (1)

(2)

(3)

(1)

J’3 A J J’4 b2 (2)

a

(3)

FIG. 1. (a) Simplified representation of distorted and nondistorted chains, chain 1 (or 3) and 2, respectively, with the J⬜ bond alternation between chains 1 and 2; (b) proposed charge order (large and small lobes represent large and small average charges) leading to a spin gap. The elementary translation (a, b) of this CO agrees with the observed periodicity of spin excitations.

© 2001 The American Physical Society

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

the alternating chains, and there would be no gap for the uniform chains. The initial NIS [3] found, however, two excitation branches, with the same gap at the antiferromagnetic (AF) point Eg1 苷 Eg2 艐 10 meV. To analyze these results, a recent spin model [12] used an explicit relation between the spin excitations and the CO. This model assumed a single gap and, as it implies zero intensity of one excitation branch, must be extended to explain the NIS data. A more precise determination of excitations in the low-T phase of NaV2 O5 is therefore crucial. In the present work, using high resolution, the dispersion of the excitations is reexplored in a wider part of the reciprocal space. Moreover, the evaluation of the structure factor, i.e., the (energy-integrated) intensity of each excitation mode, allows us to determine the charge transfer Dc . The single crystal (艐8 3 5 3 2 mm3 ) was grown by a flux method. The NIS measurements were performed at T # 4.2 K, on two thermal neutron three-axes spectrometers — IN8 and CRG/CEA-IN22 — at the Institut Laue-Langevin (ILL). On IN8, vertically focusing monochromator PG(002) and Cu(111) were used in conjunction with a vertically focusing analyzer PG(002) and horizontal collimations 600 -400 -600 . The final wave vector was kept fixed at kf 苷 4.1 Å21 . IN22 was operated at kf 苷 2.662 Å21 , with a PG(002) monochromator and a PG(002) analyzer used in a horizontal monochromatic focusing condition [resulting wave-vector resolution: dq 艐 0.03 r.l.u. (reciprocal lattice units)] with no collimation. The sample was installed in an “orange” ILL cryostat, with the scattering wave vector Q lying in the reciprocal (aⴱ , b ⴱ ) ladder plane. The two branches characterizing the low-energy excitations in NaV2 O5 have distinct energy gaps: Eg1 ﬁ Eg2 . This important result will be established when we consider the dispersions in the transverse a direction. First, however, we determine the dispersion in the leg direction (b axis). Examples of constant-energy scans obtained on IN8 as a function of Qb are displayed in Fig. 2a (wave-vector components are expressed in r.l.u.). Increasing the energy, one resolves the single peak seen at 10 meV into propagating modes (dashed lines), whose peak position is shown in Fig. 2b. They describe the dispersion of the elementary excitations in the b direction, near the AF chain wavevector component QbAF 共⬅ Qb 苷 0.5兲 . They are compared to a dispersion law characteristic of a gapped spin chain: q 2 2 E 2 兲 sin2 共2pQ 兲, where E and E共qb 兲 苷 Eg2 1 共Em b g g Em are the gap and maximum energies of the dispersion, respectively. For both Eg 苷 Eg1 , Eg2 (the solid and dashed lines, respectively), we evaluate Em 苷 93 6 6 meV. Compared to the prediction for a uniform Heisenberg chain, Em 苷 pJb 兾2, where Jb is the exchange in the chain, one obtains for the low-T phase, Jb 艐 60 meV. Second, we consider the dispersions in the aⴱ direction (i.e., along the rungs). A few examples of energy scans performed on IN22 at constant Q are reported in Fig. 3. In general, two peaks are observed. At a few Qa values, however, an extinction occurs. This extinction may

25 JUNE 2001

FIG. 2. IN8 data: (a) Constant-energy scans as a function of Qb . The full lines are the results of fits to the data, which take into account both the magnetic contributions (shown as the dashed lines) and the background (the dotted line); (b) energy dispersion in the b direction. The lines correspond to the two branches with gaps Eg1 and Eg2 .

concern one of the two modes, or the two modes simultaneously. The left and right panels report data obtained for QbAF 苷 0.5 and Qb 苷 1 (equivalent to the zone center of the AF chains QbZC ). As examples, we show for QbAF that the smallest energy difference between the two observed peaks is obtained for integer Qa values (here, Qa 苷 3), the largest one for half-integer values (Qa 苷 2.5), and an extinction of the two modes occurs at Qa 艐 1.75 (identical results have been obtained for Qb 苷 1.5). Surprisingly, at the chain zone center QbZC we found a small but nonzero intensity for the two excitation branches. The smallest energy difference between the two peaks is now obtained for half-integer values (here, Qa 苷 1.5). Extinction of one of the two modes is observed at Qa 苷 1 (on the high-energy mode) and at Qa 苷 2 (on the low-energy mode). For all the spectra recorded on IN22, the background (the dotted lines in Fig. 3) was carefully determined. Several procedures have been used involving data recorded at low and high temperatures (i.e., above Tc ). In Fig. 3a, for instance, the open dots used to define the background are obtained from measurements performed at 40 K [13] while

FIG. 3. IN12 data: Constant-Q scans as functions of energy. (a) At Qb ⬅ QbAF ; (b) at Qb ⬅ QbZC . The two arrows point to the positions expected for the two missing peaks. Curves are described in text.

5967

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

in Fig. 1b, it is determined from Qb scans performed at low temperature for different energies. For the analysis, we assume the two observed peaks to belong to two distinct contributions. Their unsymmetrical line shape is characteristic of gapped excitations undergoing a rapid energy dispersion (as established in Fig. 2b). In such a case, a dynamical response function (shown by the dashed lines in Fig. 3) is well suited to fitting, conveniently defined with only three parameters: the peak energy E1 共E2 兲 , an intensity factor A1 共A2 兲, and an energy damping G [14]. As G is mainly fixed by the resolution conditions, it is assumed to be the same for the two contributions (G 艐 0.4 0.8 meV). Together with the background, the agreement with the experiments, shown by the solid lines, is good. The values obtained for E6 as a function of Qa are shown in Fig. 4. We establish several new features. At both QbAF (open symbols) and QbZC (solid symbols), the transverse dispersion consists of two distinct excitation branches which never cross. This justifies our previous statement, namely, that there are two distinct energy gaps, Eg1 and Eg2 . In each branch, the periodicity is 2pQa : this is twice that previously determined. The two dispersions have the same amplitude, dJ 艐 1 meV but, remarkably, the upper and lower branches are out of phase, and there is phase inversion between branches at QbZC and QbAF . For each excitation AF branch, the corresponding structure factors, Sb6 共Qa 兲 and ZC Sb6 共Qa 兲 are evaluated by integrating the fitted dynamical response functions over a wide energy range (from 0 up to E 艐 300G). We estimate systematic error for varying the upper cutoff alters the results by at most 5%. The resulting values (dots and squares) are reported in Figs. 5a AF AF and 5b. The sums SbAF 共Qa 兲 苷 Sb1 共Qa 兲 1 Sb2 共Qa 兲 and ZC ZC ZC Sb 共Qa 兲 苷 Sb1 共Qa 兲 1 Sb2 共Qa 兲 are shown as the stars. The interpretation of these results is developed in three steps. First, the charge order: each spin is associated with an electronic wave function on the two sites of a rung that depends on n6 . The structure factors for the in-line

FIG. 4. Dispersion of the two excitation branches in the a direction at QbAF and QbZC . The curves are theoretical predictions fitted to the data (see text).

5968

25 JUNE 2001

and zigzag models are SQb 共Qa , v兲 苷 cos2 共pQa r兲 3 ˜ a 1 1 , Qb , v兲 and ˜ a , Qb , v兲 1 Dc2 sin2 共pQa r兲S共Q S共Q 2 ˜ a , Qb , v兲 1 Dc2 sin2 共p 3 SQb 共Qa , v兲 苷 cos2 共pQa r兲S共Q ˜ a 1 12 , Qb 1 12 , v兲, Qa r兲S共Q respectively, with v 苷 E兾h¯ and where r 苷 l兾a 艐 0.304 (l, rung length ˜ a , Qb , v兲 is the strucand a, lattice parameter), and S共Q ture factor for spins localized on the center of each rung [15]. From the ratios of intensities for different values of momentum, one can extract the charge transfer Dc inde˜ In particular, we verify that the pendent of the form of S. order cannot be in line but predictions agree with a zigzag order with Dc2 艐 0.35, i.e., Dc 艐 0.6. The agreement is particularly good for the sums SbAF 共Qa 兲 and SbZC 共Qa 兲. For the absolute intensities, we need an explicit form for S˜ which we take from the strongly dimerized limit (SDL), in which the wave function is simply a product of singlets on the stronger bonds. For the in-line model, for example, the SDL would give zero intensity at QbZC in contradiction with the observation (the data in Fig. 5b). The in-line model can be ruled out. In Figs. 5a and 5b, the predictions provided by the zigzag model (solid lines) are compared with the experimental total structure factors SbAF 共Qa 兲 and SbZC 共Qa 兲 (solid and open stars). In Fig. 5a, the agreement is obtained with no adjustable parameter except for an overall amplitude factor. Once this factor is determined, the results in Fig. 5b depend only on D2c . As can be seen, a good agreement is obtained for D2c 艐 0.35. The low-T phase of NaV2 O5 is very well described by the zigzag model, with a rather large charge transfer.

ZC AF FIG. 5. Structure factors Sb6 共Qa 兲 and Sb6 共Qa 兲 for the two magnetic branches in the a direction: (a) at QbAF ; (b) at QbZC . The solid and open stars represent the sums SbAF 共Qa 兲 and SbZC 共Qa 兲. The data are corrected from the V41 atomic form factor fV 41 , being all normalized at Qb 苷 0.5. The dot-dashed line gives the Qa dependence of fV 41 . The other curves are theoretical predictions compared to the experiments (see text).

VOLUME 86, NUMBER 26

PHYSICAL REVIEW LETTERS

Second, we consider the transverse dispersions. Later, we explain that the gap is induced by the CO. In fact, there are two distinct gaps because of the strucA tural distortions (implying distinct couplings Jb1,2 and B Jb1,2 as shown in Fig. 1b). Because of the CO, four different interchain exchange integrals must be considered, J10 , J20 , J30 , and J40 . The two branches (associated with the gaps Eg1 and Eg2 ) acquire a transverse disAF 苷 共Eg1 1 persion, described at QbAF and QbZC by Eb6 q

ZC 苷 共Eg1 2 Eg2 兲2 兾4 1 dJ 2 sin2共pQa 兲 and Eb6 q 共Eg1 1 Eg2 兲兾2 6 共Eg1 2 Eg2 兲2 兾4 1 dJ 2 cos2共pQa 兲, respectively, with dJ 苷 J10 2 J20 1 J30 2 J40 [15]. In Fig. 4, these predictions (solid and dashed lines) are compared to the data. Again, a very good agreement is obtained yielding the following evaluation Eg1 苷 10.1 6 0.1, Eg2 苷 9.1 6 0.1 and dJ 苷 1.2 6 0.1 meV. The dispersion gives directly the alternation in the interladder diagonal bonds dJ. If we assume it is dominated by the CO, we can also estimate the average from dJ 艐 J⬜ Dc2 [12] giving J⬜ 艐 2.4 meV. The structure factors can be calculated for each branch. Within the SDL approach, one obtains the contributions ZC AF Sb6 共Qa 兲 and Sb6 共Qa 兲 [16] shown by the dotted and dashed lines in Fig. 5. In Fig. 5b, the agreement with the data is rather good. In particular, the extinction phenomenon observed for each branch is well reproduced. In Fig. 5a, while the sum SbAF 共Qa 兲 is well described, we note a discrepancy between the SDL predictions and the AF AF individual structure factors Sb1 共Qa 兲 and Sb2 共Qa 兲. This difficulty could be explained as follows. As shown in Fig. 1b, two successive chains are not identical. A charge transfer giving different average valence on the chains will mix intensities at QbAF without affecting the fluctuations at QbZC in qualitative agreement with the observation [17]. Experimental supports for such a charge transfer would be useful. Our proposition for the charge ordering, i.e., the zigzag model sketched in Fig. 1a, and our estimate Dc 艐 0.6 are based on the total intensities. Finally, we consider the origin of the gap. As discussed in the introduction, the lattice distortion alone, in isolated ladders, cannot explain the presence of two energy gaps and their size. To analyze the effects of the diagonal couplings J⬜ , we refer to Fig. 1b. Each ladder is seen to be a succession of two distinct clusters (shown by ovals in the figure). By exact diagonalization of each cluster, using the effective parameters of a t-J model [10] and adding a potential imposing a charge transfer, we evaluated Jb1 and Jb2 as a function of Dc and the bond alternation d 苷 jJb1 2 Jb2 j兾共Jb1 1 Jb2 兲. For Dc 艐 0.6, the couplings underestimate the experimental value by a factor of about 2, but as the parameters calculated on the high temperature structure [10] and as such cluster calculations are rather crude, the agreement is satisfac-

Eg2 兲兾2 6

25 JUNE 2001

tory. The value obtained for the bond alternation can be considered as reasonable: d 艐 0.025 0.030. Then, using the experimental value Jb 艐 60 meV, one finds an energy gap Eg 艐 6 8 meV. This is in fairly good agreement with the experimental value Eg 艐 10 meV. This simple analysis supports the view that, in NaV2 O5 , the gaps are primarily due to the CO [18]. The lattice distortion plays a secondary role, explaining why two distinct branches are observed experimentally, and their separation. In our picture, the magnetic anisotropies are unnecessary [7]. In conclusion, the CO in NaV2 O5 is quantitatively determined by the present NIS measurements [19]. It explains also the energy gaps observed in the low-T phase of this compound.

[1] [2] [3] [4] [5]

[6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17]

[18]

[19]

M. Isobe and Y. Ueda, J. Phys. Soc. Jpn. 65, 1178 (1996). T. Chatterji et al., Solid State Commun. 108, 23 (1998). T. Yosihama et al., J. Phys. Soc. Jpn. 67, 744 (1998). S. G. Bompadre et al., cond-mat/9911298. M. Mostovoy and D. Khomski, cond-mat/9806215; A. Damascelli et al., Phys. Rev. Lett. 81, 918 (1998); P. Thalmeier and P. Fulde, Europhys. Lett. 44, 142 (1998); H. Seo and K. Fukuyama, J. Phys. Soc. Jpn. 67, 2602 (1998); J. Riera et al., Phys. Rev. B 59, 2667 (1999); A. I. Smirnov et al., ibid. 59, 14 546 (1999); H. Schwenk et al., ibid. 60, 9194 (1999); M. Lohmann et al., Phys. Rev. Lett. 85, 1742 (2000). T. Ohama et al., Phys. Rev. B 59, 3299 (1999). P. Thalmeier and A. N. Yaresko, Eur. J. Phys. B 14, 495 (2000). P. A. Carpy and J. Galy, Acta Crystallogr. Sect. B 31, 1481 (1975). H. Smolinski et al., Phys. Rev. Lett. 80, 5164 (1998). N. Suaud and M. B. Lepetit, Phys. Rev. B 62, 402 (2000). J. Lüdecke et al., Phys. Rev. Lett. 82, 3633 (1999). C. Gros and R. Valenti, Phys. Rev. Lett. 82, 976 (1999). Taking into account an estimated magnetic contribution for this temperature. T. E. Mason et al., Phys. Rev. Lett. 69, 490 (1992). O. Cepas, Ph.D. thesis, Université J. Fourier Grenoble I, France, 2000. The corresponding expressions agree with the sum rules SbAF 共Qa 兲 and SbZC 共Qa 兲 established above. In contrast, if we assume different values of Dc on two successive chains, the individual modes will mix at QbZC rather than at QbAF unlike what is observed. In T. Ohama et al., cond-mat/0003141, the CO proposed in model Z2 (Fig. 3) does not give rise to energy gaps; model Z3 provides a gap for only one out of two chains, and model Z1 is magnetically equivalent to ours (Fig. 1b). Other models assuming three different valence states (V41 , V4.51 , and V51 ) have been shown to be incompatible with our results: S. Trebst et al., Phys. Rev. B 62, R14 613 (2000); C. Gros et al., ibid. 62, R14 617 (2000), and references therein.

5969